#------------------------------------------------------------------------------
#$Date: 2016-02-20 02:53:41 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176768 $
#$URL: svn://www.crystallography.net/cod/cif/2/10/42/2104257.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2104257
loop_
_publ_author_name
'Cadoni, Marcella'
'Bloise, Andrea'
'Ferraris, Giovanni'
'Merlino, Stefano'
_publ_section_title
;
 Order--disorder character and twinning in the structure of a new
 synthetic titanosilicate: (Ba,Sr)₄Ti₆Si₄O₂₄·H₂O
;
_journal_coeditor_code           CK5034
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              669
_journal_page_last               675
_journal_paper_doi               10.1107/S0108768108032631
_journal_volume                  64
_journal_year                    2008
_chemical_formula_moiety         '(Ba,Sr)4 Ti6 Si4 O24 (H2 O)'
_chemical_formula_sum            'Ba4 H2 O25 Si4 Ti6'
_chemical_formula_weight         1351.14
_chemical_name_common
'Tetrabarium Hexatitanium Tetrasilicate Monohydrate'
_chemical_name_systematic
'Tetrabarium Hexatitanium Tetrasilicate Monohydrate'
_space_group_IT_number           65
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2 2'
_symmetry_space_group_name_H-M   'C m m m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   5.906(2)
_cell_length_b                   20.618(8)
_cell_length_c                   16.719(6)
_cell_measurement_reflns_used    1411
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.87
_cell_measurement_theta_min      1.22
_cell_volume                     2035.9(13)
_computing_molecular_graphics    'ATOMS 6.2'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker-AXS Smart Apex'
_diffrn_measurement_method       phi/omega
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.3385
_diffrn_reflns_av_sigmaI/netI    0.1445
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            10044
_diffrn_reflns_theta_full        27.87
_diffrn_reflns_theta_max         27.87
_diffrn_reflns_theta_min         1.22
_exptl_absorpt_coefficient_mu    10.180
_exptl_absorpt_correction_T_max  0.9050
_exptl_absorpt_correction_T_min  0.3626
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker SADABS'
_exptl_crystal_colour            'opaque grey'
_exptl_crystal_density_diffrn    4.408
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prismatic
_exptl_crystal_F_000             2456
_exptl_crystal_size_max          0.13
_exptl_crystal_size_mid          0.01
_exptl_crystal_size_min          0.01
_refine_diff_density_max         3.695
_refine_diff_density_min         -4.119
_refine_ls_extinction_coef       0.0015(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.041
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     96
_refine_ls_number_reflns         1411
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.041
_refine_ls_R_factor_all          0.1700
_refine_ls_R_factor_gt           0.0886
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0966P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1955
_refine_ls_wR_factor_ref         0.2388
_reflns_number_gt                692
_reflns_number_total             1411
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ck5034.cif
_cod_data_source_block           I
_cod_database_code               2104257
_cod_database_fobs_code          2104257
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'x, -y, -z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'x+1/2, -y+1/2, -z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'-x, y, z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'-x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
Ba Ba1 0.0000 0.09937(9) 0.12451(13) 0.0129(6) Uani d S 1
Ba Ba2 0.2426(4) 0.15065(17) 0.3758(2) 0.0241(8) Uani d P 0.50
Ti Ti1 0.2500 0.2500 0.0000 0.008(2) Uani d S 1
Ti Ti2 0.5000 0.0000 0.5000 0.010(3) Uani d S 1
Ti Ti3 0.0000 0.0000 0.5000 0.013(3) Uani d S 1
Ti Ti4 0.0000 0.2601(3) -0.1978(4) 0.0138(15) Uani d S 1
Ti Ti5 0.7571(12) 0.0000 0.3017(5) 0.033(3) Uani d S 1
Si Si1 0.252(3) -0.1380(9) 0.5000 0.014(4) Uiso d SP 0.50
Si Si2 -0.2500 0.2500 -0.3676(11) 0.014(4) Uiso d SP 0.50
Si Si3 0.5000 0.0000 0.1336(6) 0.002(2) Uiso d S 1
Si Si4 0.5000 0.1113(5) 0.0000 0.006(2) Uiso d S 1
O O1 0.5000 0.0638(11) 0.0769(13) 0.011(5) Uiso d S 1
O O2 0.0000 0.2444(10) -0.0780(16) 0.008(6) Uiso d S 1
O O3 0.5000 0.0633(15) 0.3053(16) 0.019(6) Uani d S 1
O O4 0.0000 0.2525(10) -0.317(2) 0.018(8) Uiso d S 1
O O5 1.0000 -0.0622(11) 0.2971(14) 0.009(5) Uiso d S 1
O O6 0.0000 -0.099(2) 0.5000 0.018(8) Uani d S 1
O O7 0.5000 -0.0969(19) 0.5000 0.015(7) Uani d S 1
O O8 0.753(3) 0.0000 0.4225(17) 0.015(8) Uani d S 1
O O9 0.250(2) 0.1875(11) -0.1991(13) 0.013(5) Uiso d . 1
O O10 0.734(3) 0.0000 0.1803(16) 0.006(6) Uiso d S 1
O O11 0.273(4) 0.1537(14) 0.0000 0.008(5) Uiso d S 1
O O12 0.246(5) 0.1849(16) 0.424(2) 0.015(7) Uiso d P 0.50
O OW1 0.0000 0.0000 0.0000 0.053(19) Uiso d S 1
O OW2 0.2500 0.2500 0.5000 0.014(13) Uiso d SP 0.50
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ti Ti 0.2776 0.4457 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O9 Ba1 O9 10 4 67.6(7)
O9 Ba1 O10 10 1_455 132.1(7)
O9 Ba1 O10 4 1_455 91.9(6)
O9 Ba1 O10 10 2_655 91.9(6)
O9 Ba1 O10 4 2_655 132.1(7)
O10 Ba1 O10 1_455 2_655 69.8(7)
O9 Ba1 O11 10 11 112.8(7)
O9 Ba1 O11 4 11 76.1(6)
O10 Ba1 O11 1_455 11 102.6(7)
O10 Ba1 O11 2_655 11 149.5(7)
O9 Ba1 O11 10 . 76.1(6)
O9 Ba1 O11 4 . 112.8(7)
O10 Ba1 O11 1_455 . 149.5(7)
O10 Ba1 O11 2_655 . 102.6(7)
O11 Ba1 O11 11 . 68.5(8)
O9 Ba1 OW1 10 . 144.6(4)
O9 Ba1 OW1 4 . 144.6(4)
O10 Ba1 OW1 1_455 . 73.6(5)
O10 Ba1 OW1 2_655 . 73.6(5)
O11 Ba1 OW1 11 . 75.9(5)
O11 Ba1 OW1 . . 75.9(5)
O9 Ba1 O5 10 2_655 73.9(6)
O9 Ba1 O5 4 2_655 73.9(6)
O10 Ba1 O5 1_455 2_655 58.7(7)
O10 Ba1 O5 2_655 2_655 58.7(7)
O11 Ba1 O5 11 2_655 143.5(4)
O11 Ba1 O5 . 2_655 143.5(4)
OW1 Ba1 O5 . 2_655 120.6(4)
O9 Ba1 O2 10 10 57.0(6)
O9 Ba1 O2 4 10 57.0(6)
O10 Ba1 O2 1_455 10 143.9(3)
O10 Ba1 O2 2_655 10 143.9(3)
O11 Ba1 O2 11 10 55.8(7)
O11 Ba1 O2 . 10 55.8(7)
OW1 Ba1 O2 . 10 120.0(5)
O5 Ba1 O2 2_655 10 119.5(7)
O9 Ba1 O1 10 1_455 143.2(5)
O9 Ba1 O1 4 1_455 75.9(5)
O10 Ba1 O1 1_455 1_455 51.3(6)
O10 Ba1 O1 2_655 1_455 116.7(5)
O11 Ba1 O1 11 1_455 51.6(6)
O11 Ba1 O1 . 1_455 115.8(5)
OW1 Ba1 O1 . 1_455 69.9(4)
O5 Ba1 O1 2_655 1_455 100.6(4)
O2 Ba1 O1 10 1_455 99.3(4)
O9 Ba1 O1 10 . 75.9(5)
O9 Ba1 O1 4 . 143.2(5)
O10 Ba1 O1 1_455 . 116.7(5)
O10 Ba1 O1 2_655 . 51.3(6)
O11 Ba1 O1 11 . 115.8(5)
O11 Ba1 O1 . . 51.6(6)
OW1 Ba1 O1 . . 69.9(4)
O5 Ba1 O1 2_655 . 100.6(4)
O2 Ba1 O1 10 . 99.3(4)
O1 Ba1 O1 1_455 . 139.8(8)
O9 Ba1 Ti4 10 10 36.3(4)
O9 Ba1 Ti4 4 10 36.3(4)
O10 Ba1 Ti4 1_455 10 125.6(4)
O10 Ba1 Ti4 2_655 10 125.6(4)
O11 Ba1 Ti4 11 10 83.4(5)
O11 Ba1 Ti4 . 10 83.4(5)
OW1 Ba1 Ti4 . 10 154.84(13)
O5 Ba1 Ti4 2_655 10 84.6(5)
O2 Ba1 Ti4 10 10 34.9(5)
O1 Ba1 Ti4 1_455 10 107.8(4)
O1 Ba1 Ti4 . 10 107.8(4)
O12 Ba2 Si2 . 7 52.5(19)
O12 Ba2 Si1 . 3_556 48.5(19)
Si2 Ba2 Si1 7 3_556 101.0(7)
O12 Ba2 O3 . . 140.8(16)
Si2 Ba2 O3 7 . 129.8(6)
Si1 Ba2 O3 3_556 . 110.0(7)
O12 Ba2 O5 . 2_655 146.4(16)
Si2 Ba2 O5 7 2_655 131.4(6)
Si1 Ba2 O5 3_556 2_655 114.7(7)
O3 Ba2 O5 . 2_655 67.8(6)
O12 Ba2 O4 . 13 77.0(18)
Si2 Ba2 O4 7 13 39.2(5)
Si1 Ba2 O4 3_556 13 116.2(8)
O3 Ba2 O4 . 13 91.0(7)
O5 Ba2 O4 2_655 13 128.9(8)
O12 Ba2 O4 . 10 77.0(18)
Si2 Ba2 O4 7 10 38.7(5)
Si1 Ba2 O4 3_556 10 118.0(8)
O3 Ba2 O4 . 10 131.8(8)
O5 Ba2 O4 2_655 10 93.7(7)
O4 Ba2 O4 13 10 66.0(3)
O12 Ba2 O6 . 9_556 72.4(19)
Si2 Ba2 O6 7 9_556 116.7(9)
Si1 Ba2 O6 3_556 9_556 38.1(5)
O3 Ba2 O6 . 9_556 112.1(10)
O5 Ba2 O6 2_655 9_556 80.1(7)
O4 Ba2 O6 13 9_556 149.4(9)
O4 Ba2 O6 10 9_556 107.4(8)
O12 Ba2 O7 . 9_656 72.1(18)
Si2 Ba2 O7 7 9_656 115.6(8)
Si1 Ba2 O7 3_556 9_656 37.0(5)
O3 Ba2 O7 . 9_656 75.4(7)
O5 Ba2 O7 2_655 9_656 112.8(9)
O4 Ba2 O7 13 9_656 105.0(7)
O4 Ba2 O7 10 9_656 149.1(9)
O6 Ba2 O7 9_556 9_656 64.4(4)
O12 Ba2 Ba2 . 11 91.2(16)
Si2 Ba2 Ba2 7 11 91.22(7)
Si1 Ba2 Ba2 3_556 11 91.5(5)
O3 Ba2 Ba2 . 11 125.2(4)
O5 Ba2 Ba2 2_655 11 57.5(3)
O4 Ba2 Ba2 13 11 124.3(3)
O4 Ba2 Ba2 10 11 58.3(3)
O6 Ba2 Ba2 9_556 11 58.5(2)
O7 Ba2 Ba2 9_656 11 122.9(2)
O12 Ba2 OW2 . . 3.3(18)
Si2 Ba2 OW2 7 . 49.2(5)
Si1 Ba2 OW2 3_556 . 51.8(5)
O3 Ba2 OW2 . . 142.1(4)
O5 Ba2 OW2 2_655 . 147.1(3)
O4 Ba2 OW2 13 . 74.5(6)
O4 Ba2 OW2 10 . 74.1(6)
O6 Ba2 OW2 9_556 . 75.0(7)
O7 Ba2 OW2 9_656 . 75.0(7)
Ba2 Ba2 OW2 11 . 90.86(5)
O12 Ba2 Ba2 . 11_655 88.8(16)
Si2 Ba2 Ba2 7 11_655 88.78(7)
Si1 Ba2 Ba2 3_556 11_655 88.5(5)
O3 Ba2 Ba2 . 11_655 54.8(4)
O5 Ba2 Ba2 2_655 11_655 122.5(3)
O4 Ba2 Ba2 13 11_655 55.7(3)
O4 Ba2 Ba2 10 11_655 121.7(3)
O6 Ba2 Ba2 9_556 11_655 121.5(2)
O7 Ba2 Ba2 9_656 11_655 57.1(2)
Ba2 Ba2 Ba2 11 11_655 180.0(3)
OW2 Ba2 Ba2 . 11_655 89.14(5)
O2 Ti1 O2 13 . 180.0000(10)
O2 Ti1 O2 13 6 82.7(12)
O2 Ti1 O2 . 6 97.3(12)
O2 Ti1 O2 13 10 97.3(12)
O2 Ti1 O2 . 10 82.7(12)
O2 Ti1 O2 6 10 180.0000(10)
O2 Ti1 O11 13 13 89.5(7)
O2 Ti1 O11 . 13 90.5(7)
O2 Ti1 O11 6 13 89.5(7)
O2 Ti1 O11 10 13 90.5(7)
O2 Ti1 O11 13 . 90.5(7)
O2 Ti1 O11 . . 89.5(7)
O2 Ti1 O11 6 . 90.5(7)
O2 Ti1 O11 10 . 89.5(7)
O11 Ti1 O11 13 . 180.0000(10)
O2 Ti1 Ti1 13 7 41.6(6)
O2 Ti1 Ti1 . 7 138.4(6)
O2 Ti1 Ti1 6 7 41.6(6)
O2 Ti1 Ti1 10 7 138.4(6)
O11 Ti1 Ti1 13 7 93.8(6)
O11 Ti1 Ti1 . 7 86.2(6)
O2 Ti1 Ti1 13 7_455 138.4(6)
O2 Ti1 Ti1 . 7_455 41.6(6)
O2 Ti1 Ti1 6 7_455 138.4(6)
O2 Ti1 Ti1 10 7_455 41.6(6)
O11 Ti1 Ti1 13 7_455 86.2(6)
O11 Ti1 Ti1 . 7_455 93.8(6)
Ti1 Ti1 Ti1 7 7_455 180.0
O2 Ti1 Ba1 13 6 48.5(6)
O2 Ti1 Ba1 . 6 131.5(6)
O2 Ti1 Ba1 6 6 91.3(6)
O2 Ti1 Ba1 10 6 88.7(6)
O11 Ti1 Ba1 13 6 41.7(4)
O11 Ti1 Ba1 . 6 138.3(4)
Ti1 Ti1 Ba1 7 6 68.451(14)
Ti1 Ti1 Ba1 7_455 6 111.549(14)
O2 Ti1 Ba1 13 13 91.3(6)
O2 Ti1 Ba1 . 13 88.7(6)
O2 Ti1 Ba1 6 13 48.5(6)
O2 Ti1 Ba1 10 13 131.5(6)
O11 Ti1 Ba1 13 13 41.7(4)
O11 Ti1 Ba1 . 13 138.3(4)
Ti1 Ti1 Ba1 7 13 68.451(14)
Ti1 Ti1 Ba1 7_455 13 111.549(14)
Ba1 Ti1 Ba1 6 13 62.38(6)
O2 Ti1 Ba1 13 10 131.5(6)
O2 Ti1 Ba1 . 10 48.5(6)
O2 Ti1 Ba1 6 10 88.7(6)
O2 Ti1 Ba1 10 10 91.3(6)
O11 Ti1 Ba1 13 10 138.3(4)
O11 Ti1 Ba1 . 10 41.7(4)
Ti1 Ti1 Ba1 7 10 111.549(14)
Ti1 Ti1 Ba1 7_455 10 68.451(14)
Ba1 Ti1 Ba1 6 10 180.00(5)
Ba1 Ti1 Ba1 13 10 117.62(6)
O2 Ti1 Ba1 13 . 88.7(6)
O2 Ti1 Ba1 . . 91.3(6)
O2 Ti1 Ba1 6 . 131.5(6)
O2 Ti1 Ba1 10 . 48.5(6)
O11 Ti1 Ba1 13 . 138.3(4)
O11 Ti1 Ba1 . . 41.7(4)
Ti1 Ti1 Ba1 7 . 111.549(14)
Ti1 Ti1 Ba1 7_455 . 68.451(14)
Ba1 Ti1 Ba1 6 . 117.62(6)
Ba1 Ti1 Ba1 13 . 180.00(5)
Ba1 Ti1 Ba1 10 . 62.38(6)
O8 Ti2 O8 10_556 2_655 180.000(2)
O8 Ti2 O8 10_556 9_656 98.2(14)
O8 Ti2 O8 2_655 9_656 81.8(14)
O8 Ti2 O8 10_556 . 81.8(14)
O8 Ti2 O8 2_655 . 98.2(14)
O8 Ti2 O8 9_656 . 180.000(3)
O8 Ti2 O7 10_556 9_656 90.000(4)
O8 Ti2 O7 2_655 9_656 90.000(4)
O8 Ti2 O7 9_656 9_656 90.000(4)
O8 Ti2 O7 . 9_656 90.000(4)
O8 Ti2 O7 10_556 . 90.000(3)
O8 Ti2 O7 2_655 . 90.000(5)
O8 Ti2 O7 9_656 . 90.000(4)
O8 Ti2 O7 . . 90.000(2)
O7 Ti2 O7 9_656 . 180.0000(10)
O8 Ti2 Ti3 10_556 . 139.1(7)
O8 Ti2 Ti3 2_655 . 40.9(7)
O8 Ti2 Ti3 9_656 . 40.9(7)
O8 Ti2 Ti3 . . 139.1(7)
O7 Ti2 Ti3 9_656 . 90.000(2)
O7 Ti2 Ti3 . . 90.000(2)
O8 Ti2 Ti3 10_556 1_655 40.9(7)
O8 Ti2 Ti3 2_655 1_655 139.1(7)
O8 Ti2 Ti3 9_656 1_655 139.1(7)
O8 Ti2 Ti3 . 1_655 40.9(7)
O7 Ti2 Ti3 9_656 1_655 90.000(2)
O7 Ti2 Ti3 . 1_655 90.000(2)
Ti3 Ti2 Ti3 . 1_655 180.0
O8 Ti2 Ba2 10_556 4_656 51.54(14)
O8 Ti2 Ba2 2_655 4_656 128.46(14)
O8 Ti2 Ba2 9_656 4_656 87.0(5)
O8 Ti2 Ba2 . 4_656 93.0(5)
O7 Ti2 Ba2 9_656 4_656 39.65(5)
O7 Ti2 Ba2 . 4_656 140.35(5)
Ti3 Ti2 Ba2 . 4_656 112.14(4)
Ti3 Ti2 Ba2 1_655 4_656 67.86(4)
O8 Ti2 Ba2 10_556 11_655 93.0(5)
O8 Ti2 Ba2 2_655 11_655 87.0(5)
O8 Ti2 Ba2 9_656 11_655 128.46(14)
O8 Ti2 Ba2 . 11_655 51.54(14)
O7 Ti2 Ba2 9_656 11_655 39.65(5)
O7 Ti2 Ba2 . 11_655 140.35(5)
Ti3 Ti2 Ba2 . 11_655 112.14(4)
Ti3 Ti2 Ba2 1_655 11_655 67.86(4)
Ba2 Ti2 Ba2 4_656 11_655 61.97(11)
O8 Ti2 Ba2 10_556 12 128.46(14)
O8 Ti2 Ba2 2_655 12 51.54(14)
O8 Ti2 Ba2 9_656 12 93.0(5)
O8 Ti2 Ba2 . 12 87.0(5)
O7 Ti2 Ba2 9_656 12 140.35(5)
O7 Ti2 Ba2 . 12 39.65(5)
Ti3 Ti2 Ba2 . 12 67.86(4)
Ti3 Ti2 Ba2 1_655 12 112.14(4)
Ba2 Ti2 Ba2 4_656 12 180.0
Ba2 Ti2 Ba2 11_655 12 118.03(11)
O8 Ti2 Ba2 10_556 10_556 87.0(5)
O8 Ti2 Ba2 2_655 10_556 93.0(5)
O8 Ti2 Ba2 9_656 10_556 51.54(14)
O8 Ti2 Ba2 . 10_556 128.46(14)
O7 Ti2 Ba2 9_656 10_556 39.65(5)
O7 Ti2 Ba2 . 10_556 140.35(5)
Ti3 Ti2 Ba2 . 10_556 67.86(4)
Ti3 Ti2 Ba2 1_655 10_556 112.14(4)
Ba2 Ti2 Ba2 4_656 10_556 44.28(8)
Ba2 Ti2 Ba2 11_655 10_556 79.29(10)
Ba2 Ti2 Ba2 12 10_556 135.72(8)
O8 Ti3 O8 9_656 1_455 180.000(2)
O8 Ti3 O8 9_656 2_655 83.3(15)
O8 Ti3 O8 1_455 2_655 96.7(15)
O8 Ti3 O8 9_656 10_456 96.7(15)
O8 Ti3 O8 1_455 10_456 83.3(15)
O8 Ti3 O8 2_655 10_456 180.000(3)
O8 Ti3 O6 9_656 9_556 90.000(4)
O8 Ti3 O6 1_455 9_556 90.000(4)
O8 Ti3 O6 2_655 9_556 90.000(4)
O8 Ti3 O6 10_456 9_556 90.000(4)
O8 Ti3 O6 9_656 . 90.000(3)
O8 Ti3 O6 1_455 . 90.000(5)
O8 Ti3 O6 2_655 . 90.000(3)
O8 Ti3 O6 10_456 . 90.000(5)
O6 Ti3 O6 9_556 . 180.0000(10)
O8 Ti3 Ti2 9_656 . 41.6(8)
O8 Ti3 Ti2 1_455 . 138.4(8)
O8 Ti3 Ti2 2_655 . 41.6(8)
O8 Ti3 Ti2 10_456 . 138.4(8)
O6 Ti3 Ti2 9_556 . 90.000(2)
O6 Ti3 Ti2 . . 90.000(2)
O8 Ti3 Ti2 9_656 1_455 138.4(8)
O8 Ti3 Ti2 1_455 1_455 41.6(8)
O8 Ti3 Ti2 2_655 1_455 138.4(8)
O8 Ti3 Ti2 10_456 1_455 41.6(8)
O6 Ti3 Ti2 9_556 1_455 90.000(2)
O6 Ti3 Ti2 . 1_455 90.000(2)
Ti2 Ti3 Ti2 . 1_455 180.0
O8 Ti3 Ba2 9_656 10_556 52.24(15)
O8 Ti3 Ba2 1_455 10_556 127.76(15)
O8 Ti3 Ba2 2_655 10_556 94.4(5)
O8 Ti3 Ba2 10_456 10_556 85.6(5)
O6 Ti3 Ba2 9_556 10_556 39.09(5)
O6 Ti3 Ba2 . 10_556 140.91(5)
Ti2 Ti3 Ba2 . 10_556 69.02(4)
Ti2 Ti3 Ba2 1_455 10_556 110.98(4)
O8 Ti3 Ba2 9_656 11 127.76(15)
O8 Ti3 Ba2 1_455 11 52.24(15)
O8 Ti3 Ba2 2_655 11 85.6(5)
O8 Ti3 Ba2 10_456 11 94.4(5)
O6 Ti3 Ba2 9_556 11 39.09(5)
O6 Ti3 Ba2 . 11 140.91(5)
Ti2 Ti3 Ba2 . 11 110.98(4)
Ti2 Ti3 Ba2 1_455 11 69.02(4)
Ba2 Ti3 Ba2 10_556 11 78.17(11)
O8 Ti3 Ba2 9_656 2 127.76(15)
O8 Ti3 Ba2 1_455 2 52.24(15)
O8 Ti3 Ba2 2_655 2 85.6(5)
O8 Ti3 Ba2 10_456 2 94.4(5)
O6 Ti3 Ba2 9_556 2 140.91(5)
O6 Ti3 Ba2 . 2 39.09(5)
Ti2 Ti3 Ba2 . 2 110.98(4)
Ti2 Ti3 Ba2 1_455 2 69.02(4)
Ba2 Ti3 Ba2 10_556 2 180.0
Ba2 Ti3 Ba2 11 2 101.83(11)
O8 Ti3 Ba2 9_656 4_556 85.6(5)
O8 Ti3 Ba2 1_455 4_556 94.4(5)
O8 Ti3 Ba2 2_655 4_556 127.76(15)
O8 Ti3 Ba2 10_456 4_556 52.24(15)
O6 Ti3 Ba2 9_556 4_556 39.09(5)
O6 Ti3 Ba2 . 4_556 140.91(5)
Ti2 Ti3 Ba2 . 4_556 110.98(4)
Ti2 Ti3 Ba2 1_455 4_556 69.02(4)
Ba2 Ti3 Ba2 10_556 4_556 41.96(8)
Ba2 Ti3 Ba2 11 4_556 62.53(11)
Ba2 Ti3 Ba2 2 4_556 138.04(8)
O9 Ti4 O9 6 16_455 107.7(13)
O9 Ti4 O4 6 . 92.0(8)
O9 Ti4 O4 16_455 . 92.0(8)
O9 Ti4 O2 6 . 96.1(8)
O9 Ti4 O2 16_455 . 96.1(8)
O4 Ti4 O2 . . 166.3(9)
O9 Ti4 O9 6 11 170.7(6)
O9 Ti4 O9 16_455 11 81.5(10)
O4 Ti4 O9 . 11 86.2(7)
O2 Ti4 O9 . 11 84.0(7)
O9 Ti4 O9 6 . 81.5(10)
O9 Ti4 O9 16_455 . 170.7(6)
O4 Ti4 O9 . . 86.2(7)
O2 Ti4 O9 . . 84.0(7)
O9 Ti4 O9 11 . 89.2(10)
O9 Ti4 Ti4 6 6_455 151.9(7)
O9 Ti4 Ti4 16_455 6_455 44.2(6)
O4 Ti4 Ti4 . 6_455 89.36(10)
O2 Ti4 Ti4 . 6_455 88.72(10)
O9 Ti4 Ti4 11 6_455 37.3(5)
O9 Ti4 Ti4 . 6_455 126.6(6)
O9 Ti4 Ti4 6 6 44.2(6)
O9 Ti4 Ti4 16_455 6 151.9(7)
O4 Ti4 Ti4 . 6 89.36(10)
O2 Ti4 Ti4 . 6 88.72(10)
O9 Ti4 Ti4 11 6 126.6(6)
O9 Ti4 Ti4 . 6 37.3(5)
Ti4 Ti4 Ti4 6_455 6 163.9(5)
O9 Ti4 Ba1 6 10 123.9(7)
O9 Ti4 Ba1 16_455 10 123.9(7)
O4 Ti4 Ba1 . 10 105.7(6)
O2 Ti4 Ba1 . 10 60.5(6)
O9 Ti4 Ba1 11 10 48.4(5)
O9 Ti4 Ba1 . 10 48.4(5)
Ti4 Ti4 Ba1 6_455 10 82.4(2)
Ti4 Ti4 Ba1 6 10 82.4(2)
O9 Ti4 Ba2 6 7_455 91.6(7)
O9 Ti4 Ba2 16_455 7_455 52.0(7)
O4 Ti4 Ba2 . 7_455 42.3(5)
O2 Ti4 Ba2 . 7_455 147.9(4)
O9 Ti4 Ba2 11 7_455 93.2(6)
O9 Ti4 Ba2 . 7_455 128.0(7)
Ti4 Ti4 Ba2 6_455 7_455 70.91(12)
Ti4 Ti4 Ba2 6 7_455 117.54(14)
Ba1 Ti4 Ba2 10 7_455 136.29(17)
O9 Ti4 Ba2 6 13 52.0(7)
O9 Ti4 Ba2 16_455 13 91.6(7)
O4 Ti4 Ba2 . 13 42.3(5)
O2 Ti4 Ba2 . 13 147.9(4)
O9 Ti4 Ba2 11 13 128.0(7)
O9 Ti4 Ba2 . 13 93.2(6)
Ti4 Ti4 Ba2 6_455 13 117.54(14)
Ti4 Ti4 Ba2 6 13 70.91(12)
Ba1 Ti4 Ba2 10 13 136.29(17)
Ba2 Ti4 Ba2 7_455 13 46.98(12)
O9 Ti4 Ba2 6 4 127.8(7)
O9 Ti4 Ba2 16_455 4 92.0(7)
O4 Ti4 Ba2 . 4 38.2(5)
O2 Ti4 Ba2 . 4 130.1(5)
O9 Ti4 Ba2 11 4 48.6(6)
O9 Ti4 Ba2 . 4 80.9(6)
Ti4 Ti4 Ba2 6_455 4 64.29(14)
Ti4 Ti4 Ba2 6 4 105.99(19)
Ba1 Ti4 Ba2 10 4 74.25(13)
Ba2 Ti4 Ba2 7_455 4 63.20(14)
Ba2 Ti4 Ba2 13 4 80.49(17)
O5 Ti5 O5 2_755 . 83.5(11)
O5 Ti5 O3 2_755 . 97.6(10)
O5 Ti5 O3 . . 178.8(9)
O5 Ti5 O3 2_755 2_655 178.8(9)
O5 Ti5 O3 . 2_655 97.6(10)
O3 Ti5 O3 . 2_655 81.3(13)
O5 Ti5 O8 2_755 . 92.8(9)
O5 Ti5 O8 . . 92.8(9)
O3 Ti5 O8 . . 87.8(9)
O3 Ti5 O8 2_655 . 87.8(9)
O5 Ti5 O10 2_755 . 90.6(8)
O5 Ti5 O10 . . 90.6(8)
O3 Ti5 O10 . . 88.8(9)
O3 Ti5 O10 2_655 . 88.8(10)
O8 Ti5 O10 . . 175.5(9)
O5 Ti5 Ti5 2_755 2_755 41.8(5)
O5 Ti5 Ti5 . 2_755 41.8(5)
O3 Ti5 Ti5 . 2_755 139.3(7)
O3 Ti5 Ti5 2_655 2_755 139.3(7)
O8 Ti5 Ti5 . 2_755 90.7(6)
O10 Ti5 Ti5 . 2_755 93.8(6)
O5 Ti5 Ti5 2_755 2_655 138.2(5)
O5 Ti5 Ti5 . 2_655 138.2(5)
O3 Ti5 Ti5 . 2_655 40.7(7)
O3 Ti5 Ti5 2_655 2_655 40.7(7)
O8 Ti5 Ti5 . 2_655 89.3(6)
O10 Ti5 Ti5 . 2_655 86.2(6)
Ti5 Ti5 Ti5 2_755 2_655 180.0000(10)
O5 Ti5 Ba2 2_755 11_655 52.8(6)
O5 Ti5 Ba2 . 11_655 129.3(6)
O3 Ti5 Ba2 . 11_655 52.0(7)
O3 Ti5 Ba2 2_655 11_655 126.5(7)
O8 Ti5 Ba2 . 11_655 68.26(14)
O10 Ti5 Ba2 . 11_655 111.69(14)
Ti5 Ti5 Ba2 2_755 11_655 89.97(13)
Ti5 Ti5 Ba2 2_655 11_655 90.03(12)
O5 Ti5 Ba2 2_755 2_655 129.3(6)
O5 Ti5 Ba2 . 2_655 52.8(6)
O3 Ti5 Ba2 . 2_655 126.5(7)
O3 Ti5 Ba2 2_655 2_655 52.0(7)
O8 Ti5 Ba2 . 2_655 68.26(14)
O10 Ti5 Ba2 . 2_655 111.69(14)
Ti5 Ti5 Ba2 2_755 2_655 89.97(13)
Ti5 Ti5 Ba2 2_655 2_655 90.03(13)
Ba2 Ti5 Ba2 11_655 2_655 136.5(3)
O5 Ti5 Ba1 2_755 1_655 48.8(7)
O5 Ti5 Ba1 . 1_655 92.6(7)
O3 Ti5 Ba1 . 1_655 87.7(7)
O3 Ti5 Ba1 2_655 1_655 130.4(8)
O8 Ti5 Ba1 . 1_655 140.2(4)
O10 Ti5 Ba1 . 1_655 42.5(4)
Ti5 Ti5 Ba1 2_755 1_655 68.28(10)
Ti5 Ti5 Ba1 2_655 1_655 111.72(10)
Ba2 Ti5 Ba1 11_655 1_655 77.99(9)
Ba2 Ti5 Ba1 2_655 1_655 140.7(2)
O5 Ti5 Ba1 2_755 2_655 92.6(7)
O5 Ti5 Ba1 . 2_655 48.8(7)
O3 Ti5 Ba1 . 2_655 130.4(8)
O3 Ti5 Ba1 2_655 2_655 87.7(7)
O8 Ti5 Ba1 . 2_655 140.2(4)
O10 Ti5 Ba1 . 2_655 42.5(4)
Ti5 Ti5 Ba1 2_755 2_655 68.28(10)
Ti5 Ti5 Ba1 2_655 2_655 111.72(10)
Ba2 Ti5 Ba1 11_655 2_655 140.7(2)
Ba2 Ti5 Ba1 2_655 2_655 77.99(9)
Ba1 Ti5 Ba1 1_655 2_655 63.80(14)
O12 Si1 O12 12 3_556 105(3)
O12 Si1 O7 12 . 108.8(14)
O12 Si1 O7 3_556 . 108.8(14)
O12 Si1 O6 12 . 105.6(14)
O12 Si1 O6 3_556 . 105.6(14)
O7 Si1 O6 . . 122(2)
O12 Si1 Ba2 12 12 30.1(12)
O12 Si1 Ba2 3_556 12 135.5(16)
O7 Si1 Ba2 . 12 94.9(5)
O6 Si1 Ba2 . 12 92.0(5)
O12 Si1 Ba2 12 3_556 135.5(16)
O12 Si1 Ba2 3_556 3_556 30.1(12)
O7 Si1 Ba2 . 3_556 94.9(5)
O6 Si1 Ba2 . 3_556 92.0(5)
Ba2 Si1 Ba2 12 3_556 165.3(10)
O12 Si1 OW2 12 3_556 52.7(13)
O12 Si1 OW2 3_556 3_556 52.7(13)
O7 Si1 OW2 . 3_556 120.3(15)
O6 Si1 OW2 . 3_556 118.0(15)
Ba2 Si1 OW2 12 3_556 82.8(5)
Ba2 Si1 OW2 3_556 3_556 82.8(5)
O12 Si1 Ba2 12 2 58.6(11)
O12 Si1 Ba2 3_556 2 113.5(13)
O7 Si1 Ba2 . 2 137.8(8)
O6 Si1 Ba2 . 2 47.1(8)
Ba2 Si1 Ba2 12 2 52.8(3)
Ba2 Si1 Ba2 3_556 2 122.8(6)
OW2 Si1 Ba2 3_556 2 85.6(4)
O12 Si1 Ba2 12 9_556 113.5(13)
O12 Si1 Ba2 3_556 9_556 58.6(11)
O7 Si1 Ba2 . 9_556 137.8(8)
O6 Si1 Ba2 . 9_556 47.1(8)
Ba2 Si1 Ba2 12 9_556 122.8(6)
Ba2 Si1 Ba2 3_556 9_556 52.8(3)
OW2 Si1 Ba2 3_556 9_556 85.6(4)
Ba2 Si1 Ba2 2 9_556 70.6(3)
O12 Si1 Ba2 12 2_655 61.4(11)
O12 Si1 Ba2 3_556 2_655 115.3(13)
O7 Si1 Ba2 . 2_655 47.7(8)
O6 Si1 Ba2 . 2_655 139.0(8)
Ba2 Si1 Ba2 12 2_655 56.5(3)
Ba2 Si1 Ba2 3_556 2_655 125.3(6)
OW2 Si1 Ba2 3_556 2_655 86.1(4)
Ba2 Si1 Ba2 2 2_655 109.33(11)
Ba2 Si1 Ba2 9_556 2_655 171.7(6)
O12 Si1 Ba2 12 9_656 115.3(13)
O12 Si1 Ba2 3_556 9_656 61.4(11)
O7 Si1 Ba2 . 9_656 47.7(8)
O6 Si1 Ba2 . 9_656 139.0(8)
Ba2 Si1 Ba2 12 9_656 125.3(6)
Ba2 Si1 Ba2 3_556 9_656 56.5(3)
OW2 Si1 Ba2 3_556 9_656 86.1(4)
Ba2 Si1 Ba2 2 9_656 171.7(6)
Ba2 Si1 Ba2 9_556 9_656 109.33(11)
Ba2 Si1 Ba2 2_655 9_656 69.5(3)
O12 Si2 O12 7_455 4 110(3)
O12 Si2 O4 7_455 . 105.9(13)
O12 Si2 O4 4 . 107.5(13)
O12 Si2 O4 7_455 6_455 107.5(13)
O12 Si2 O4 4 6_455 105.9(13)
O4 Si2 O4 . 6_455 120(2)
O12 Si2 Ba2 7_455 7_455 31.2(12)
O12 Si2 Ba2 4 7_455 141.1(16)
O4 Si2 Ba2 . 7_455 91.2(7)
O4 Si2 Ba2 6_455 7_455 92.6(7)
O12 Si2 Ba2 7_455 4 141.1(16)
O12 Si2 Ba2 4 4 31.2(12)
O4 Si2 Ba2 . 4 92.6(7)
O4 Si2 Ba2 6_455 4 91.2(7)
Ba2 Si2 Ba2 7_455 4 172.4(11)
O12 Si2 OW2 7_455 7_455 54.9(13)
O12 Si2 OW2 4 7_455 54.9(13)
O4 Si2 OW2 . 7_455 120.0(11)
O4 Si2 OW2 6_455 7_455 120.0(11)
Ba2 Si2 OW2 7_455 7_455 86.2(5)
Ba2 Si2 OW2 4 7_455 86.2(5)
O12 Si2 Ba2 7_455 13_455 59.7(10)
O12 Si2 Ba2 4 13_455 117.4(11)
O4 Si2 Ba2 . 13_455 135.2(9)
O4 Si2 Ba2 6_455 13_455 47.9(8)
Ba2 Si2 Ba2 7_455 13_455 53.57(10)
Ba2 Si2 Ba2 4 13_455 126.07(13)
OW2 Si2 Ba2 7_455 13_455 87.8(3)
O12 Si2 Ba2 7_455 10 117.4(11)
O12 Si2 Ba2 4 10 59.7(10)
O4 Si2 Ba2 . 10 47.9(8)
O4 Si2 Ba2 6_455 10 135.2(9)
Ba2 Si2 Ba2 7_455 10 126.07(13)
Ba2 Si2 Ba2 4 10 53.57(10)
OW2 Si2 Ba2 7_455 10 87.8(3)
Ba2 Si2 Ba2 13_455 10 175.6(6)
O12 Si2 Ba2 7_455 13 61.8(10)
O12 Si2 Ba2 4 13 115.4(11)
O4 Si2 Ba2 . 13 44.6(8)
O4 Si2 Ba2 6_455 13 138.6(10)
Ba2 Si2 Ba2 7_455 13 56.81(11)
Ba2 Si2 Ba2 4 13 122.85(13)
OW2 Si2 Ba2 7_455 13 87.8(3)
Ba2 Si2 Ba2 13_455 13 110.38(10)
Ba2 Si2 Ba2 10 13 69.44(10)
O12 Si2 Ba2 7_455 10_455 115.4(11)
O12 Si2 Ba2 4 10_455 61.8(10)
O4 Si2 Ba2 . 10_455 138.6(10)
O4 Si2 Ba2 6_455 10_455 44.6(8)
Ba2 Si2 Ba2 7_455 10_455 122.85(13)
Ba2 Si2 Ba2 4 10_455 56.81(11)
OW2 Si2 Ba2 7_455 10_455 87.8(3)
Ba2 Si2 Ba2 13_455 10_455 69.45(10)
Ba2 Si2 Ba2 10 10_455 110.38(10)
Ba2 Si2 Ba2 13 10_455 175.7(6)
O10 Si3 O10 . 2_655 121.2(19)
O10 Si3 O1 . . 106.7(6)
O10 Si3 O1 2_655 . 106.7(6)
O10 Si3 O1 . 2_655 106.7(6)
O10 Si3 O1 2_655 2_655 106.7(6)
O1 Si3 O1 . 2_655 108.5(17)
O10 Si3 Ba1 . 1_655 46.0(6)
O10 Si3 Ba1 2_655 1_655 137.4(6)
O1 Si3 Ba1 . 1_655 60.9(3)
O1 Si3 Ba1 2_655 1_655 115.9(4)
O10 Si3 Ba1 . 2 137.4(6)
O10 Si3 Ba1 2_655 2 46.0(6)
O1 Si3 Ba1 . 2 115.9(4)
O1 Si3 Ba1 2_655 2 60.9(3)
Ba1 Si3 Ba1 1_655 2 175.2(3)
O10 Si3 Ba1 . . 137.4(6)
O10 Si3 Ba1 2_655 . 46.0(6)
O1 Si3 Ba1 . . 60.9(3)
O1 Si3 Ba1 2_655 . 115.9(4)
Ba1 Si3 Ba1 1_655 . 110.35(6)
Ba1 Si3 Ba1 2 . 69.43(6)
O10 Si3 Ba1 . 2_655 46.0(6)
O10 Si3 Ba1 2_655 2_655 137.4(6)
O1 Si3 Ba1 . 2_655 115.9(4)
O1 Si3 Ba1 2_655 2_655 60.9(3)
Ba1 Si3 Ba1 1_655 2_655 69.43(6)
Ba1 Si3 Ba1 2 2_655 110.35(6)
Ba1 Si3 Ba1 . 2_655 175.2(3)
O11 Si4 O11 11_655 . 114(2)
O11 Si4 O1 11_655 10 109.3(6)
O11 Si4 O1 . 10 109.3(6)
O11 Si4 O1 11_655 . 109.3(6)
O11 Si4 O1 . . 109.3(6)
O1 Si4 O1 10 . 105.4(17)
O11 Si4 Ba1 11_655 10 136.1(6)
O11 Si4 Ba1 . 10 49.7(6)
O1 Si4 Ba1 10 10 60.1(3)
O1 Si4 Ba1 . 10 114.6(4)
O11 Si4 Ba1 11_655 1_655 49.7(6)
O11 Si4 Ba1 . 1_655 136.1(6)
O1 Si4 Ba1 10 1_655 114.6(4)
O1 Si4 Ba1 . 1_655 60.1(3)
Ba1 Si4 Ba1 10 1_655 172.2(3)
O11 Si4 Ba1 11_655 10_655 49.7(6)
O11 Si4 Ba1 . 10_655 136.1(6)
O1 Si4 Ba1 10 10_655 60.1(3)
O1 Si4 Ba1 . 10_655 114.6(4)
Ba1 Si4 Ba1 10 10_655 109.26(7)
Ba1 Si4 Ba1 1_655 10_655 70.18(6)
O11 Si4 Ba1 11_655 . 136.1(6)
O11 Si4 Ba1 . . 49.7(6)
O1 Si4 Ba1 10 . 114.6(4)
O1 Si4 Ba1 . . 60.1(3)
Ba1 Si4 Ba1 10 . 70.18(6)
Ba1 Si4 Ba1 1_655 . 109.26(7)
Ba1 Si4 Ba1 10_655 . 172.2(3)
Si4 O1 Si3 . . 163.0(16)
Si4 O1 Ba1 . 1_655 93.4(5)
Si3 O1 Ba1 . 1_655 92.4(5)
Si4 O1 Ba1 . . 93.4(5)
Si3 O1 Ba1 . . 92.4(5)
Ba1 O1 Ba1 1_655 . 139.8(8)
Ti1 O2 Ti1 . 7_455 96.9(12)
Ti1 O2 Ti4 . . 130.0(6)
Ti1 O2 Ti4 7_455 . 130.0(6)
Ti1 O2 Ba1 . 10 102.9(7)
Ti1 O2 Ba1 7_455 10 102.9(7)
Ti4 O2 Ba1 . 10 84.6(8)
Ti5 O3 Ti5 2_655 . 98.6(13)
Ti5 O3 Ba2 2_655 11_655 153.7(13)
Ti5 O3 Ba2 . 11_655 91.2(4)
Ti5 O3 Ba2 2_655 . 91.2(4)
Ti5 O3 Ba2 . . 153.7(13)
Ba2 O3 Ba2 11_655 . 70.5(8)
Si2 O4 Si2 . 11 120(2)
Si2 O4 Ti4 . . 120.0(11)
Si2 O4 Ti4 11 . 120.0(11)
Si2 O4 Ba2 . 13 109.1(13)
Si2 O4 Ba2 11 13 49.5(5)
Ti4 O4 Ba2 . 13 107.9(9)
Si2 O4 Ba2 . 7_455 49.5(5)
Si2 O4 Ba2 11 7_455 109.1(13)
Ti4 O4 Ba2 . 7_455 107.9(9)
Ba2 O4 Ba2 13 7_455 68.6(6)
Si2 O4 Ba2 . 4 48.8(5)
Si2 O4 Ba2 11 4 104.5(12)
Ti4 O4 Ba2 . 4 115.0(9)
Ba2 O4 Ba2 13 4 137.1(13)
Ba2 O4 Ba2 7_455 4 98.1(6)
Si2 O4 Ba2 . 10 104.5(12)
Si2 O4 Ba2 11 10 48.8(5)
Ti4 O4 Ba2 . 10 115.0(9)
Ba2 O4 Ba2 13 10 98.1(6)
Ba2 O4 Ba2 7_455 10 137.1(13)
Ba2 O4 Ba2 4 10 63.4(5)
Ti5 O5 Ti5 2_755 . 96.3(11)
Ti5 O5 Ba2 2_755 2_655 146.7(11)
Ti5 O5 Ba2 . 2_655 92.0(4)
Ti5 O5 Ba2 2_755 12_655 92.0(4)
Ti5 O5 Ba2 . 12_655 146.7(11)
Ba2 O5 Ba2 2_655 12_655 65.0(5)
Ti5 O5 Ba1 2_755 2_655 102.1(8)
Ti5 O5 Ba1 . 2_655 102.1(8)
Ba2 O5 Ba1 2_655 2_655 107.5(7)
Ba2 O5 Ba1 12_655 2_655 107.5(7)
Si1 O6 Si1 11 . 123(3)
Si1 O6 Ti3 11 . 118.3(14)
Si1 O6 Ti3 . . 118.3(14)
Si1 O6 Ba2 11 2 49.8(4)
Si1 O6 Ba2 . 2 106.0(13)
Ti3 O6 Ba2 . 2 112.9(8)
Si1 O6 Ba2 11 12 106.0(13)
Si1 O6 Ba2 . 12 49.8(4)
Ti3 O6 Ba2 . 12 112.9(8)
Ba2 O6 Ba2 2 12 63.1(4)
Si1 O6 Ba2 11 3_556 106.0(13)
Si1 O6 Ba2 . 3_556 49.8(4)
Ti3 O6 Ba2 . 3_556 112.9(8)
Ba2 O6 Ba2 2 3_556 134.3(16)
Ba2 O6 Ba2 12 3_556 98.7(8)
Si1 O6 Ba2 11 9_556 49.8(4)
Si1 O6 Ba2 . 9_556 106.0(13)
Ti3 O6 Ba2 . 9_556 112.9(8)
Ba2 O6 Ba2 2 9_556 98.7(8)
Ba2 O6 Ba2 12 9_556 134.3(16)
Ba2 O6 Ba2 3_556 9_556 63.1(4)
Si1 O7 Si1 . 11_655 120(3)
Si1 O7 Ti2 . . 120.0(13)
Si1 O7 Ti2 11_655 . 120.0(13)
Si1 O7 Ba2 . 12 48.1(4)
Si1 O7 Ba2 11_655 12 105.8(13)
Ti2 O7 Ba2 . 12 113.3(7)
Si1 O7 Ba2 . 2_655 105.8(13)
Si1 O7 Ba2 11_655 2_655 48.1(4)
Ti2 O7 Ba2 . 2_655 113.3(7)
Ba2 O7 Ba2 12 2_655 65.7(4)
Si1 O7 Ba2 . 9_656 105.8(13)
Si1 O7 Ba2 11_655 9_656 48.1(4)
Ti2 O7 Ba2 . 9_656 113.3(7)
Ba2 O7 Ba2 12 9_656 133.4(15)
Ba2 O7 Ba2 2_655 9_656 95.7(7)
Si1 O7 Ba2 . 3_556 48.1(4)
Si1 O7 Ba2 11_655 3_556 105.8(13)
Ti2 O7 Ba2 . 3_556 113.3(7)
Ba2 O7 Ba2 12 3_556 95.7(7)
Ba2 O7 Ba2 2_655 3_556 133.4(15)
Ba2 O7 Ba2 9_656 3_556 65.7(4)
Ti3 O8 Ti2 1_655 . 97.5(13)
Ti3 O8 Ti5 1_655 . 131.0(12)
Ti2 O8 Ti5 . . 131.6(11)
Ti3 O8 Ba2 1_655 11_655 99.0(4)
Ti2 O8 Ba2 . 11_655 99.5(4)
Ti5 O8 Ba2 . 11_655 75.9(5)
Ti3 O8 Ba2 1_655 2_655 99.0(4)
Ti2 O8 Ba2 . 2_655 99.5(4)
Ti5 O8 Ba2 . 2_655 75.9(5)
Ba2 O8 Ba2 11_655 2_655 151.7(10)
Ti4 O9 Ti4 6 . 98.4(10)
Ti4 O9 Ba1 6 10 148.0(11)
Ti4 O9 Ba1 . 10 95.3(6)
Ti4 O9 Ba2 6 10 99.8(8)
Ti4 O9 Ba2 . 10 100.2(8)
Ba1 O9 Ba2 10 10 106.0(7)
Si3 O10 Ti5 . . 123.2(13)
Si3 O10 Ba1 . 1_655 109.4(9)
Ti5 O10 Ba1 . 1_655 107.5(7)
Si3 O10 Ba1 . 2_655 109.4(9)
Ti5 O10 Ba1 . 2_655 107.5(7)
Ba1 O10 Ba1 1_655 2_655 96.6(7)
Si4 O11 Ti1 . . 126.9(14)
Si4 O11 Ba1 . 10 104.9(10)
Ti1 O11 Ba1 . 10 110.7(7)
Si4 O11 Ba1 . . 104.9(10)
Ti1 O11 Ba1 . . 110.7(7)
Ba1 O11 Ba1 10 . 93.4(7)
Ba2 O12 Si1 . 3_556 101(2)
Ba2 O12 Si2 . 7 96(2)
Si1 O12 Si2 3_556 7 162(3)
Ba2 O12 Ba2 . 11 68.5(15)
Si1 O12 Ba2 3_556 11 95.1(14)
Si2 O12 Ba2 7 11 92.9(13)
Ba2 O12 Ba2 . 11_655 71.6(15)
Si1 O12 Ba2 3_556 11_655 92.6(13)
Si2 O12 Ba2 7 11_655 91.4(12)
Ba2 O12 Ba2 11 11_655 140.1(12)
Ba1 OW1 Ba1 10 . 90.91(9)
Ba1 OW1 Ba1 10 9 89.09(9)
Ba1 OW1 Ba1 . 9 180.00(8)
Ba1 OW1 Ba1 10 2 180.00(5)
Ba1 OW1 Ba1 . 2 89.09(9)
Ba1 OW1 Ba1 9 2 90.91(9)
Si2 OW2 Si2 7 11_556 180.000(2)
Si2 OW2 Si1 7 15 90.000(2)
Si2 OW2 Si1 11_556 15 90.000(2)
Si2 OW2 Si1 7 3_556 90.000(2)
Si2 OW2 Si1 11_556 3_556 90.000(2)
Si1 OW2 Si1 15 3_556 180.000(3)
Si2 OW2 Ba2 7 6 44.61(7)
Si2 OW2 Ba2 11_556 6 135.39(7)
Si1 OW2 Ba2 15 6 45.41(7)
Si1 OW2 Ba2 3_556 6 134.59(7)
Si2 OW2 Ba2 7 . 44.61(7)
Si2 OW2 Ba2 11_556 . 135.39(7)
Si1 OW2 Ba2 15 . 134.59(7)
Si1 OW2 Ba2 3_556 . 45.41(7)
Ba2 OW2 Ba2 6 . 89.22(14)
Si2 OW2 Ba2 7 13_556 135.39(7)
Si2 OW2 Ba2 11_556 13_556 44.61(7)
Si1 OW2 Ba2 15 13_556 45.41(7)
Si1 OW2 Ba2 3_556 13_556 134.59(7)
Ba2 OW2 Ba2 6 13_556 90.78(14)
Ba2 OW2 Ba2 . 13_556 180.00(10)
Si2 OW2 Ba2 7 10_556 135.39(7)
Si2 OW2 Ba2 11_556 10_556 44.61(7)
Si1 OW2 Ba2 15 10_556 134.59(7)
Si1 OW2 Ba2 3_556 10_556 45.41(7)
Ba2 OW2 Ba2 6 10_556 180.0
Ba2 OW2 Ba2 . 10_556 90.78(14)
Ba2 OW2 Ba2 13_556 10_556 89.22(14)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Ba1 O9 10 2.65(2)
Ba1 O9 4 2.654(19)
Ba1 O10 1_455 2.744(14)
Ba1 O10 2_655 2.744(14)
Ba1 O11 11 2.860(16)
Ba1 O11 . 2.860(16)
Ba1 OW1 . 2.921(2)
Ba1 O5 2_655 2.99(2)
Ba1 O2 10 3.09(2)
Ba1 O1 1_455 3.145(8)
Ba1 O1 . 3.145(8)
Ba1 Ti4 10 3.534(7)
Ba2 O12 . 1.07(3)
Ba2 Si2 7 2.053(4)
Ba2 Si1 3_556 2.094(4)
Ba2 O3 . 2.63(2)
Ba2 O5 2_655 2.67(2)
Ba2 O4 13 2.70(2)
Ba2 O4 10 2.73(2)
Ba2 O6 9_556 2.738(16)
Ba2 O7 9_656 2.802(16)
Ba2 Ba2 11 2.865(5)
Ba2 OW2 . 2.917(4)
Ba2 Ba2 11_655 3.041(5)
Ti1 O2 13 1.973(18)
Ti1 O2 . 1.973(18)
Ti1 O2 6 1.973(18)
Ti1 O2 10 1.973(18)
Ti1 O11 13 1.99(3)
Ti1 O11 . 1.99(3)
Ti1 Ti1 7 2.9530(10)
Ti1 Ti1 7_455 2.9530(10)
Ti1 Ba1 6 4.020(2)
Ti1 Ba1 13 4.020(2)
Ti1 Ba1 10 4.020(2)
Ti2 O8 10_556 1.98(2)
Ti2 O8 2_655 1.98(2)
Ti2 O8 9_656 1.98(2)
Ti2 O8 . 1.98(2)
Ti2 O7 9_656 2.00(4)
Ti2 O7 . 2.00(4)
Ti2 Ti3 . 2.9530(10)
Ti2 Ti3 1_655 2.9530(10)
Ti2 Ba2 4_656 4.034(4)
Ti2 Ba2 11_655 4.034(4)
Ti2 Ba2 12 4.034(4)
Ti2 Ba2 10_556 4.034(3)
Ti3 O8 9_656 1.95(2)
Ti3 O8 1_455 1.95(2)
Ti3 O8 2_655 1.95(2)
Ti3 O8 10_456 1.95(2)
Ti3 O6 9_556 2.04(4)
Ti3 O6 . 2.04(4)
Ti3 Ti2 1_455 2.9530(10)
Ti3 Ba2 10_556 4.002(4)
Ti3 Ba2 11 4.002(3)
Ti3 Ba2 2 4.002(4)
Ti3 Ba2 4_556 4.002(3)
Ti4 O9 6 1.828(18)
Ti4 O9 16_455 1.828(18)
Ti4 O4 . 1.99(3)
Ti4 O2 . 2.03(3)
Ti4 O9 11 2.103(19)
Ti4 O9 . 2.103(19)
Ti4 Ti4 6_455 2.982(2)
Ti4 Ti4 6 2.982(2)
Ti4 Ba1 10 3.534(7)
Ti4 Ba2 7_455 3.814(7)
Ti4 Ba2 13 3.814(7)
Ti4 Ba2 4 4.000(7)
Ti5 O5 2_755 1.925(16)
Ti5 O5 . 1.925(16)
Ti5 O3 . 2.00(2)
Ti5 O3 2_655 2.00(2)
Ti5 O8 . 2.02(3)
Ti5 O10 . 2.03(3)
Ti5 Ti5 2_755 2.869(14)
Ti5 Ti5 2_655 3.037(14)
Ti5 Ba2 11_655 3.344(5)
Ti5 Ba2 2_655 3.344(5)
Ti5 Ba1 1_655 3.877(7)
Ti5 Ba1 2_655 3.877(7)
Si1 O12 12 1.60(3)
Si1 O12 3_556 1.60(3)
Si1 O7 . 1.69(2)
Si1 O6 . 1.69(3)
Si1 Ba2 12 2.094(4)
Si1 Ba2 3_556 2.094(4)
Si1 OW2 3_556 2.310(18)
Si1 Ba2 2 3.594(13)
Si1 Ba2 9_556 3.594(13)
Si1 Ba2 2_655 3.645(14)
Si1 Ba2 9_656 3.645(14)
Si2 O12 7_455 1.64(3)
Si2 O12 4 1.64(3)
Si2 O4 . 1.706(19)
Si2 O4 6_455 1.706(19)
Si2 Ba2 7_455 2.053(4)
Si2 Ba2 4 2.053(4)
Si2 OW2 7_455 2.214(19)
Si2 Ba2 13_455 3.561(3)
Si2 Ba2 10 3.561(3)
Si2 Ba2 13 3.632(3)
Si2 Ba2 10_455 3.633(3)
Si3 O10 . 1.59(2)
Si3 O10 2_655 1.59(2)
Si3 O1 . 1.62(2)
Si3 O1 2_655 1.62(2)
Si3 Ba1 1_655 3.5973(15)
Si3 Ba1 2 3.5973(15)
Si3 Ba1 2_655 3.5973(15)
Si4 O11 11_655 1.60(3)
Si4 O11 . 1.60(3)
Si4 O1 10 1.62(2)
Si4 O1 . 1.62(2)
Si4 Ba1 10 3.6214(17)
Si4 Ba1 1_655 3.6214(17)
Si4 Ba1 10_655 3.6214(17)
O1 Ba1 1_655 3.145(8)
O2 Ti1 7_455 1.973(18)
O2 Ba1 10 3.09(2)
O3 Ti5 2_655 2.00(2)
O3 Ba2 11_655 2.63(2)
O4 Si2 11 1.706(19)
O4 Ba2 13 2.70(2)
O4 Ba2 7_455 2.70(2)
O4 Ba2 4 2.73(2)
O4 Ba2 10 2.73(2)
O5 Ti5 2_755 1.925(16)
O5 Ba2 2_655 2.67(2)
O5 Ba2 12_655 2.67(2)
O5 Ba1 2_655 2.99(2)
O6 Si1 11 1.69(3)
O6 Ba2 2 2.738(16)
O6 Ba2 12 2.738(16)
O6 Ba2 3_556 2.738(16)
O6 Ba2 9_556 2.738(16)
O7 Si1 11_655 1.69(2)
O7 Ba2 12 2.802(16)
O7 Ba2 2_655 2.802(16)
O7 Ba2 9_656 2.802(16)
O7 Ba2 3_556 2.802(16)
O8 Ti3 1_655 1.95(2)
O8 Ba2 11_655 3.203(8)
O8 Ba2 2_655 3.203(8)
O9 Ti4 6 1.828(18)
O9 Ba1 10 2.654(19)
O9 Ba2 10 3.05(2)
O10 Ba1 1_655 2.744(14)
O10 Ba1 2_655 2.744(14)
O11 Ba1 10 2.860(16)
O12 Si1 3_556 1.60(3)
O12 Si2 7 1.64(3)
O12 Ba2 11 3.08(3)
O12 Ba2 11_655 3.20(3)
OW1 Ba1 10 2.921(2)
OW1 Ba1 9 2.921(2)
OW1 Ba1 2 2.921(2)
OW2 Si2 7 2.214(19)
OW2 Si2 11_556 2.214(19)
OW2 Si1 15 2.310(18)
OW2 Si1 3_556 2.310(18)
OW2 Ba2 6 2.917(4)
OW2 Ba2 13_556 2.917(4)
OW2 Ba2 10_556 2.917(4)
